#------------------------------------------------------------------------------
#$Date: 2019-11-22 22:24:58 +0200 (Fri, 22 Nov 2019) $
#$Revision: 231424 $
#$URL: file:///home/coder/svn-repositories/cod/cif/4/00/31/4003197.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4003197
loop_
_publ_author_name
'McKellar, Scott C.'
'Sotelo, Jorge'
'Greenaway, Alex'
'Mowat, John P. S.'
'Kvam, Odin'
'Morrison, Carole A.'
'Wright, Paul A.'
'Moggach, Stephen A.'
_publ_section_title
;
 Pore Shape Modification of a Microporous Metal--Organic Framework Using
 High Pressure: Accessing a New Phase with Oversized Guest Molecules
;
_journal_issue                   2
_journal_name_full               'Chemistry of Materials'
_journal_page_first              466
_journal_paper_doi               10.1021/acs.chemmater.5b02891
_journal_volume                  28
_journal_year                    2016
_chemical_formula_moiety         'C24 H12 O12 Sc2'
_chemical_formula_sum            'C24 H12 O12 Sc2'
_chemical_formula_weight         582.26
_space_group_IT_number           70
_space_group_name_Hall           '-F 2uv 2vw'
_space_group_name_H-M_alt        'F d d d :2'
_symmetry_cell_setting           orthorhombic
_symmetry_Int_Tables_number      70
_symmetry_space_group_name_Hall  '-F 2uv 2vw'
_symmetry_space_group_name_H-M   'F d d d :2'
_atom_sites_solution_hydrogens   difmap
_atom_sites_solution_primary     other
_audit_creation_date             15-06-08
_audit_creation_method           CRYSTALS_ver_14.40
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.7578(9)
_cell_length_b                   20.7293(11)
_cell_length_c                   34.292(3)
_cell_measurement_reflns_used    1850
_cell_measurement_temperature    293
_cell_measurement_theta_max      22
_cell_measurement_theta_min      4
_cell_volume                     6225.5(9)
_computing_cell_refinement       'Apex2 (Bruker AXS, 2006)'
_computing_data_collection       'Apex2 (Bruker AXS, 2006)'
_computing_data_reduction        'Apex2 (Bruker AXS, 2006)'
_computing_molecular_graphics    'CAMERON (Watkin et al., 1996)'
_computing_publication_material  'CRYSTALS (Betteridge et al., 2003)'
_computing_structure_refinement  'CRYSTALS (Betteridge et al., 2003)'
_computing_structure_solution    'USER DEFINED STRUCTURE SOLUTION'
_diffrn_ambient_pressure         200000
_diffrn_ambient_temperature      293
_diffrn_measured_fraction_theta_full 0.733
_diffrn_measured_fraction_theta_max 0.686
_diffrn_measurement_device       Area
_diffrn_measurement_device_type  'Bruker Kappa Apex2'
_diffrn_measurement_method       ω
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.083
_diffrn_reflns_limit_h_max       7
_diffrn_reflns_limit_h_min       -7
_diffrn_reflns_limit_k_max       21
_diffrn_reflns_limit_k_min       -21
_diffrn_reflns_limit_l_max       32
_diffrn_reflns_limit_l_min       -31
_diffrn_reflns_number            3979
_diffrn_reflns_theta_full        16.200
_diffrn_reflns_theta_max         21.600
_diffrn_reflns_theta_min         3.803
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    0.487
_exptl_absorpt_correction_T_max  0.95
_exptl_absorpt_correction_T_min  0.78
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS (Siemens, 1996)'
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    1.242
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             2352
_exptl_crystal_size_max          0.200
_exptl_crystal_size_mid          0.100
_exptl_crystal_size_min          0.100
_refine_diff_density_max         0.72
_refine_diff_density_min         -0.47
_refine_ls_extinction_coef       8.524
_refine_ls_extinction_method     'Larson (1970), Equation 22'
_refine_ls_goodness_of_fit_ref   1.0082
_refine_ls_hydrogen_treatment    noref
_refine_ls_matrix_type           full
_refine_ls_number_parameters     97
_refine_ls_number_reflns         625
_refine_ls_number_restraints     101
_refine_ls_R_factor_all          0.0742
_refine_ls_R_factor_gt           0.0523
_refine_ls_shift/su_max          0.0014452
_refine_ls_shift/su_mean         0.0000812
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
;
 Method= Modified Sheldrick 
 w=1/[σ²(F²) + ( 0.05P)² +99.12P] 
 ,where P=(max(Fo²,0) + 2Fc²)/3 
;
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_all         0.1222
_refine_ls_wR_factor_gt          0.1141
_refine_ls_wR_factor_ref         0.1222
_reflns_limit_h_max              7
_reflns_limit_h_min              0
_reflns_limit_k_max              21
_reflns_limit_k_min              0
_reflns_limit_l_max              32
_reflns_limit_l_min              0
_reflns_number_gt                463
_reflns_number_total             629
_reflns_threshold_expression     I>2.0σ(I)
_oxford_diffrn_Wilson_B_factor   0.00
_oxford_diffrn_Wilson_scale      0.00
_oxford_refine_ls_r_factor_ref   0.0742
_oxford_refine_ls_scale          0.05312(3)
_oxford_reflns_number_all        625
_oxford_reflns_threshold_expression_ref I>-3.0\s(I)
_oxford_structure_analysis_title 'ST4046s in Fddd'
_cod_data_source_file            cm5b02891_si_003.cif
_cod_data_source_block           SC2BDC3_mh_I
_cod_depositor_comments
;
The following automatic conversions were performed:

data item '_atom_sites_solution_primary' value 'Other' was changed to
'other' in accordance with the
/home/saulius/struct/COD-crude-data/automatic-downloads/DataCite-retrospective/ACS/depositions/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 last updated on
2011-04-26.

Automatic conversion script
Id: cif_fix_values 6909 2019-04-08 15:41:33Z antanas 
;
_cod_original_sg_symbol_H-M      'F d d d'
_cod_database_code               4003197
_iucr_refine_instruction_details_constraints
;
#
# Punched on 08/06/15 at 11:50:58
#
#LIST     12                                                                    
BLOCK X'S 
CONT SCALE 
CONT SC   (1 ,U'S)  UNTIL C(8) 
END                                                                             
;
_iucr_refine_instruction_details_restraints
;
#
# Punched on 08/06/15 at 11:50:58
#
#LIST     16                                                                    
NO 
DIST 1.39, 0.01 = C(2) TO C(3) 
DIST 1.39, 0.01 = C(3) TO C(4) 
DIST 1.39, 0.01 = C(2,-1,4,0,0,1) TO C(4) 
DIST 1.39, 0.01 = C(6) TO C(7) 
DIST 1.39, 0.01 = C(7) TO C(8) 
DIST 1.39, 0.01 = C(8) TO C(6,-2,1,0,1,1) 
ANGLE 120, 1 = C(2) TO C(3) TO C(4) 
ANGLE 120, 1 = C(1) TO C(2) TO C(3) 
ANGLE 120, 1 = C(4,-1,4,0,0,1) TO C(2) TO C(3) 
ANGLE 120, 1 = C(7) TO C(8) TO C(6,-2,1,0,1,1) 
ANGLE 120, 1 = C(6) TO C(7) TO C(8) 
ANGLE 120, 1 = C(5) TO C(6) TO  C(7) 
PLANAR 0.010000  C(6) C(7) C(8)  C(6,-2,1,0,1,1) 
PLANAR 0.010000  C(2,-1,4,0,0,1) C(2) C(3) C(4) 
REM   DELU   START (DO NOT REMOVE THIS LINE) 
VIBR .0, 0.00200 = O(1) TO C(1) 
VIBR .0, 0.00200 = O(2) TO C(1) 
VIBR .0, 0.00200 = O(3) TO C(5) 
VIBR .0, 0.00200 = C(1) TO C(2) 
VIBR .0, 0.00500 = O(1) TO O(2) 
VIBR .0, 0.00500 = C(2) TO O(2) 
VIBR .0, 0.00500 = C(2) TO O(1) 
VIBR .0, 0.00200 = C(2) TO C(4,-1,4,0,0,1) 
VIBR .0, 0.00200 = C(2) TO C(3) 
VIBR .0, 0.00500 = C(4,-1,4,0,0,1) TO C(1) 
VIBR .0, 0.00500 = C(3) TO C(1) 
VIBR .0, 0.00500 = C(3) TO C(4,-1,4,0,0,1) 
VIBR .0, 0.00200 = C(3) TO C(4) 
VIBR .0, 0.00500 = C(4) TO C(2) 
VIBR .0, 0.00500 = C(2,-1,4,0,0,1) TO C(3) 
VIBR .0, 0.00200 = C(5) TO C(6) 
VIBR .0, 0.00500 = O(3,-3,1,0,0,1) TO O(3) 
VIBR .0, 0.00500 = C(6) TO O(3) 
VIBR .0, 0.00500 = C(6) TO O(3,-3,1,0,0,1) 
VIBRATION 0.0, 0.020000 = C(6) TO C(7) 
VIBRATION 0.0, 0.020000 = C(7) TO C(8) 
VIBRATION 0.0, 0.050000 = C(6) TO C(8) 
VIBRATION 0.0, 0.050000 = C(5) TO C(7) 
REM   DELU   END (DO NOT REMOVE THIS LINE) 
REM   THERMSIM   START (DO NOT REMOVE THIS LINE) 
U(IJ) .0, 0.08000 = O(1) TO C(1) 
U(IJ) .0, 0.08000 = O(2) TO C(1) 
U(IJ) .0, 0.04000 = O(3) TO C(5) 
U(IJ) .0, 0.04000 = C(1) TO C(2) 
U(IJ) .0, 0.04000 = C(2) TO C(4,-1,4,0,0,1) 
U(IJ) .0, 0.04000 = C(2) TO C(3) 
U(IJ) .0, 0.04000 = C(3) TO C(4) 
U(IJ) .0, 0.04000 = C(5) TO C(6) 
U(IJ)'S  0.0, 0.010000 = C(7) TO C(8) 
U(IJ)'S  0.0, 0.010000 = C(6) TO C(7) 
REM   THERMSIM   END (DO NOT REMOVE THIS LINE) 
END                                                                             
;
loop_
_symmetry_equiv_pos_as_xyz
x,y,z
-x,-y,-z
x,y+1/2,z+1/2
-x,-y+1/2,-z+1/2
x+1/2,y,z+1/2
-x+1/2,-y,-z+1/2
x+1/2,y+1/2,z
-x+1/2,-y+1/2,-z
-x,y+1/4,z+1/4
x,-y+1/4,-z+1/4
-x,y+3/4,z+3/4
x,-y+3/4,-z+3/4
-x+1/2,y+1/4,z+3/4
x+1/2,-y+1/4,-z+3/4
-x+1/2,y+3/4,z+1/4
x+1/2,-y+3/4,-z+1/4
x+1/4,-y,z+1/4
-x+1/4,y,-z+1/4
x+1/4,-y+1/2,z+3/4
-x+1/4,y+1/2,-z+3/4
x+3/4,-y,z+3/4
-x+3/4,y,-z+3/4
x+3/4,-y+1/2,z+1/4
-x+3/4,y+1/2,-z+1/4
-x+1/4,-y+3/4,z+1/2
x+1/4,y+3/4,-z+1/2
-x+1/4,-y+5/4,z+1
x+1/4,y+5/4,-z+1
-x+3/4,-y+3/4,z+1
x+3/4,y+3/4,-z+1
-x+3/4,-y+5/4,z+1/2
x+3/4,y+5/4,-z+1/2
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_occupancy
_atom_site_adp_type
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
Sc1 Sc 0.3750 0.3750 0.63561(5) 0.0152 1.0000 Uani S T
O1 O 0.2457(7) 0.3342(2) 0.59289(14) 0.0504 1.0000 Uani . U
O2 O 0.0087(7) 0.3335(2) 0.57019(12) 0.0394 1.0000 Uani . U
O3 O 0.2452(7) 0.45798(18) 0.63555(15) 0.0460 1.0000 Uani . U
C1 C 0.1463(11) 0.3204(3) 0.5675(2) 0.0327 1.0000 Uani D U
C2 C 0.2005(7) 0.2835(2) 0.53225(16) 0.0354 1.0000 Uani D U
C3 C 0.0961(7) 0.2634(3) 0.50490(17) 0.0593 1.0000 Uani D U
C4 C 0.1460(9) 0.2300(3) 0.47213(18) 0.0622 1.0000 Uani D U
C5 C 0.1250 0.4855(4) 0.6250 0.0342 1.0000 Uani DS TU
C6 C 0.1250 0.5579(3) 0.6250 0.0464 1.0000 Uani DS TU
C7 C 0.2579(9) 0.5910(5) 0.6345(3) 0.0470 0.5000 Uani D U
C8 C 0.2580(10) 0.6584(5) 0.6340(3) 0.0511 0.5000 Uani D U
H3 H -0.0089 0.2736 0.5078 0.0723 1.0000 Uiso . .
H4 H 0.0748 0.2174 0.4524 0.0760 1.0000 Uiso . .
H7 H 0.3482 0.5680 0.6410 0.0543 0.5000 Uiso . .
H8 H 0.3490 0.6813 0.6403 0.0585 0.5000 Uiso . .
loop_
_atom_type_symbol
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_Cromer_Mann_a1
_atom_type_scat_Cromer_Mann_b1
_atom_type_scat_Cromer_Mann_a2
_atom_type_scat_Cromer_Mann_b2
_atom_type_scat_Cromer_Mann_a3
_atom_type_scat_Cromer_Mann_b3
_atom_type_scat_Cromer_Mann_a4
_atom_type_scat_Cromer_Mann_b4
_atom_type_scat_Cromer_Mann_c
_atom_type_scat_source
C 0.0033 0.0016 2.3100 20.8439 1.0200 10.2075 1.5886 0.5687 0.8650 51.6512
0.2156 'International Tables Vol C 4.2.6.8 and 6.1.1.4'
H 0.0000 0.0000 0.4930 10.5109 0.3229 26.1257 0.1402 3.1424 0.0408 57.7998
0.0030 'International Tables Vol C 4.2.6.8 and 6.1.1.4'
O 0.0106 0.0060 3.0485 13.2771 2.2868 5.7011 1.5463 0.3239 0.8670 32.9089
0.2508 'International Tables Vol C 4.2.6.8 and 6.1.1.4'
Sc 0.2519 0.3716 9.1890 9.0213 7.3679 0.5729 1.6409 136.1080 1.4680 51.3531
1.3329 'International Tables Vol C 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_site_symmetry_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_3
_geom_angle
_geom_angle_publ_flag
O2 16_556 Sc1 O2 18_556 87.6(3) yes
O2 16_556 Sc1 O3 29_554 92.0(2) yes
O2 18_556 Sc1 O3 29_554 88.1(2) yes
O2 16_556 Sc1 O1 29_554 92.2(2) yes
O2 18_556 Sc1 O1 29_554 179.7(2) yes
O3 29_554 Sc1 O1 29_554 92.2(2) yes
O2 16_556 Sc1 O1 . 179.7(2) yes
O2 18_556 Sc1 O1 . 92.2(2) yes
O3 29_554 Sc1 O1 . 87.7(2) yes
O1 29_554 Sc1 O1 . 87.9(3) yes
O2 16_556 Sc1 O3 . 88.1(2) yes
O2 18_556 Sc1 O3 . 92.0(2) yes
O3 29_554 Sc1 O3 . 179.9(3) yes
O1 29_554 Sc1 O3 . 87.7(2) yes
O1 . Sc1 O3 . 92.2(2) yes
Sc1 . O1 C1 . 166.7(5) yes
Sc1 16_456 O2 C1 . 133.3(4) yes
Sc1 . O3 C5 . 147.7(5) yes
O1 . C1 O2 . 124.6(7) yes
O1 . C1 C2 . 116.8(7) yes
O2 . C1 C2 . 118.5(6) yes
C1 . C2 C4 8_556 119.8(6) yes
C1 . C2 C3 . 119.5(5) yes
C4 8_556 C2 C3 . 120.8(5) yes
C2 . C3 C4 . 119.6(5) yes
C2 . C3 H3 . 120.4 no
C4 . C3 H3 . 119.9 no
C3 . C4 C2 8_556 119.6(6) yes
C3 . C4 H4 . 120.2 no
C2 8_556 C4 H4 . 120.2 no
O3 . C5 O3 18_556 125.7(8) yes
O3 . C5 C6 . 117.2(4) yes
O3 18_556 C5 C6 . 117.2(4) yes
C5 . C6 C8 27_554 120.1(5) yes
C5 . C6 C8 10_566 120.1(5) yes
C8 27_554 C6 C8 10_566 119.7(10) yes
C5 . C6 C7 18_556 119.6(5) yes
C8 27_554 C6 C7 18_556 26.3(5) yes
C8 10_566 C6 C7 18_556 113.6(6) yes
C5 . C6 C7 . 119.6(5) yes
C8 27_554 C6 C7 . 113.6(6) yes
C8 10_566 C6 C7 . 26.3(5) yes
C7 18_556 C6 C7 . 120.7(9) yes
C7 10_566 C7 C6 . 110.6(5) yes
C7 10_566 C7 H8 10_566 92.9 no
C6 . C7 H8 10_566 101.1 no
C7 10_566 C7 C8 . 24.1(5) yes
C6 . C7 C8 . 119.5(7) yes
H8 10_566 C7 C8 . 111.1 no
C7 10_566 C7 H7 . 123.7 no
C6 . C7 H7 . 120.2 no
H8 10_566 C7 H7 . 56.4 no
C8 . C7 H7 . 120.2 no
C8 10_566 C8 C7 . 24.7(5) yes
C8 10_566 C8 C6 27_554 111.6(6) yes
C7 . C8 C6 27_554 120.2(7) yes
C8 10_566 C8 H7 10_566 94.3 no
C7 . C8 H7 10_566 113.3 no
C6 27_554 C8 H7 10_566 100.1 no
C8 10_566 C8 H8 . 123.2 no
C7 . C8 H8 . 119.8 no
C6 27_554 C8 H8 . 120.0 no
H7 10_566 C8 H8 . 55.8 no
C7 . H7 C8 10_566 29.1 no
C8 . H8 C7 10_566 29.6 no
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_2
_geom_bond_distance
_geom_bond_publ_flag
Sc1 O2 16_556 2.100(5) yes
Sc1 O2 18_556 2.100(5) yes
Sc1 O3 29_554 2.062(4) yes
Sc1 O1 29_554 2.035(5) yes
Sc1 O1 . 2.035(5) yes
Sc1 O3 . 2.062(4) yes
O1 C1 . 1.265(9) yes
O2 C1 . 1.239(9) yes
O3 C5 . 1.251(6) yes
C1 C2 . 1.506(8) yes
C2 C4 8_556 1.382(7) yes
C2 C3 . 1.375(7) yes
C3 C4 . 1.390(6) yes
C3 H3 . 0.949 no
C4 H4 . 0.956 no
C5 C6 . 1.499(11) yes
C6 C8 27_554 1.394(8) yes
C6 C8 10_566 1.394(8) yes
C6 C7 18_556 1.390(8) yes
C6 C7 . 1.390(8) yes
C7 C7 10_566 1.55(2) yes
C7 H8 10_566 1.253 no
C7 C8 . 1.397(7) yes
C7 H7 . 0.951 no
C8 C8 10_566 1.52(2) yes
C8 H7 10_566 1.266 no
C8 H8 . 0.951 no
